Microstructural Evolution and Phase Transformation in ...· Microstructural Evolution and Phase...
Embed Size (px)
Transcript of Microstructural Evolution and Phase Transformation in ...· Microstructural Evolution and Phase...
DOI: http://dx.doi.org/10.1590/1980-5373-MR-2016-0560Materials Research. 2018; 21(1): e20160560
Microstructural Evolution and Phase Transformation in Laser Cladding of Cr and Mo Powder on Grey Cast Iron: Mixture Design of Experiment (DOE)
Abd Rahman Zulhishamuddina*, Reza Mohamed Suffiana, Syarifah Nur Aqidaa,b,
Maarof Mohd Rashidia
Received: July 27, 2016; Revised: March 09, 2017; Accepted: October 18, 2017
Laser cladding on grey cast iron at high power processing was investigated for microstructural evolution and phase transformation to enhance surface properties. Cladding was designed using a mixture of DOE with peak power (Pp) and pulse repetition frequency (PRF), and a mixture component of Cr and Mo ratio as factors. Microstructural findings indicated absolute elimination of graphite phase from the clad zone, in conjunction with particles evolution occurrence. Meanwhile, Cr, Mo and Fe phases were detected on the clad surface, along with M-C carbide, retained austenite and MoFe formation. The clad surface with addition of Mo exhibited a high hardness value of 945.5 HV0.1 due to carbide formation. As a result of high peak power penetration into substrate surface, the depth range of clad zone was 53 to 131 m. From the optimisation, the highest desirability is 82.3 %. Cladding with molybdenum powder addition was found to have produced minimum surface roughness, maximum depth and hardness of 9.14 m, 110 m and 891.1 HV0.1, respectively.
Keywords: Graphite, grey cast iron, laser cladding.
Recent advances in materials design emphasise or focus on sustainability and low cost consumption. Conventional material, such as grey cast iron, is among the cheapest and common engineering materials with a wide range of applications in automotive components such as break disc and cylinder liner. Previous reports from the industry and a number of research have shown that these automotive parts usually experience certain defects such as wear, corrosion and thermal wear1. The operational conditions of these parts include elevated temperature, high pressure and sliding friction, which contribute to multifaceted, high-stress condition2. Meanwhile, failure of the components made of grey cast iron occurred near-surface graphite phase which acted as a source of crack nucleation under impact condition and caused crack growth. In automotive application, cylinder liner of engines experiences high friction at an elevated temperature that requires such properties to prevent crack and increase the life of cylinder liner. In long-cycle operation, high wear rate leads to corrosion and produces sulphur in the fuel during operation3. Therefore, elimination of graphite phase near the surface is an option. With the presence of hard phase on the surface, corrosion and wear can be avoided4.
Laser cladding is a process where the added material is deposited onto the substrate with the purpose to improve the properties of the substrate. This process can be achieved by using either laser beam or arc as the heat source to melt
the added material during deposition onto the surface of the substrate. In laser cladding, addition of fine particles like Cr and Mo on the substrate surface resulted in enhanced strength, hardness and wear resistance5,6. A previous report showed that modifying surface using tungsten inert gas (TIG) in cast iron surface alloyed with chromium and molybdenum formed the structure of cementite, martensite, as well as retained austenite and primary carbides structure of (Fe,Cr)7C3 and (Fe,Mo)3C5. As a result, the alloyed surfaces have higher hardness compared to the melting surface because of the carbide formation. Though a lot of works have been conducted on laser cladding of grey cast iron to enhance the hardness and wear resistance using carbon and Fe-based powder7,8, there is limited research conducted on laser cladding on grey cast iron surfaced with chromium and molybdenum powder since considerable free carbon, in the form of graphite flakes, is present and laser surface modification on cast iron is challenging9. Thus, this research aims to study surface modification of grey cast iron by pre-placing chromium, molybdenum and mixture between them on the grey cast iron using laser cladding. This study also aims to optimise laser processing to enhance cylinder liner life and prevent premature failure of friction due to high temperature.
2. Materials and Methods
As-received grey cast iron was cut into samples of 40 mm diameter and 10 mm thickness. The chemical
aFaculty of Mechanical Engineering, Universiti Malaysia Pahang, 26600, Pekan Pahang, MalaysiabAutomotive Engineering Centre, Universiti Malaysia Pahang, 26600, Pekan Pahang, Malaysia
Zulhishamuddin et al.2 Materials Research
composition of the as-received grey cast iron is shown in Table 1, whereas Figure 1 shows the microstructure of the as-received grey cast iron. The structure shows that graphite lamella is surrounded with -ferrite and pearlite. The average hardness for this material is 278.5 HV0.1. Cr and Mo powders of 99.9 % purity, with the particle size range of 71.9 to 130 m and 0.969 to 9.62 m respectively, were used. These powders were mixed with a bonding agent called sodium silicate prior to pre-placement on grey cast iron substrate surface. The pre-placed powders were dried in a furnace at the temperature of 200oC for 2 h. This technique is to bind the powders and prevent them from being dispersed during laser processing10,7. The thickness of the pre-placed powder layer was in the range of 0.3 to 0.7 mm as the alloying component had the maximum penetration amount in the thickness of coating11.
A comprehensive experiment that combines a mixture of components with process factor was used to design laser cladding of grey cast iron with the addition of Cr and Mo particles. The combined mixture components design of experiment was developed at two numerical factor and mixture component at two levels to yield 12 parameter settings. The mixture components were Cr and Mo, while peak power (PP) and pulse repetition frequency (PRF) were the process factors. Three responses were depth of molten zone, surface roughness and hardness. The outcome parameters from the setting were pulse energy (EP), residence time (TR) and irradiance (I). Setting the parameter at different values was found to produce significant amounts of energy and irradiance to melt and clad the sample at laser spot size of 1 mm. The design was optimised for minimum surface roughness and maximum surface depth and hardness.
Laser processing was conducted using JK300HPS Nd:YAG twin lamp laser source pulse TEM00 mode, 50 W average power, 1064 nm wavelength at the laser spot size of 1 mm. The laser cladding parameters were peak power in range of 800 to 1200 W, pulse repetition frequency in range of 80 to 90 Hz and the scan speed in the range of 2.4 to 21.6 mms-1. During the laser processing, surface of the sample was heated up from room temperature to its melting temperature. Meanwhile, the cooling period (tcooling) of the sample was determined from the 'off' state duration of the laser pulse (see Equation 1). Hence, the cooling rate (CR) can be calculated as per Equation 2.
Table 1. Chemical composition for as-received grey cast iron.
Material C Si Mn P S Fe
Grey cast iron 3.55 1.58 0.76 0.09 0.08 Bal.
Figure 1. Microstucture as-received of grey cast iron at 500 magnification.
Where, T is temperature deviation from room temperature to the melting temperature. The parameter setting and outcome parameters are summarised in Table 2. The sample was placed on the table with linear movement translated by CNC moving control system. In order to prevent oxidation, laser processing was assisted by argon gas in constant flow at 10 Lmin-1.
Metallographic study was carried out using IM7000 Series Inverted Optical microscopes with Progress Capture 28.8 Jenoptik Optical System image analyser software and scanning electron microscopes (SEM). The modified surface roughness was determined using the 2D stylus profilometer model Mitutoyo SJ-410 series. X-ray diffractometer model Rigaku Miniflex with Cu K was generated at 30 kV and current of 15 mA, while a scanning range of 3 to 80 was used to analyse presence of the phase in the modified surface. Meanwhile, the PDXL analysis software was used to identify the phase from the x-ray diffraction result. The range of penetration depth (1/e) for some substances in Cu K is 0.1 to 10 m, which is in the range of a typical layer thickness12. Hardness properties were measured using MMT Matsuzawa Vickers Hardness tester with 100 gf load. The experimental results were statistically analysed by using the ANOVA approach to establish the relationship between the factors and responses.
3. Results and Discussion
The metallographic study revealed a clad layer formation on the grey cast iron substrate, as shown in Figure 2. The micrographs of modified sample cross section in Figure 2 indicate the presence of clad zone, interface zone and substrate material. The clad zone depth is 127 m, 131 m and 96
CR t Tcooling=D
t Tcooling PRF R1= -
3Microstructural Evolution and Phase Transformation in Laser Cladding of Cr and Mo Powder on Grey Cast Iron: Mixture Design of Experiment (DOE)
Table 2. Parameter settings for laser surface cladding of grey cast iron.
Input parameter Outcome
Pp PRF Pave V Ep TR I
% % W Hz W mm/s J s W/mm2
1 100 0 800 80
19.2 0.63 0.0033
2 100 0 800 90 21.6 0.56 0.0029
3 100 0 1200 80 19.2 0.63 0.0022
4 100 0 1200 90 21.6 0.56 0.0019
5 0 100 800 80 19.2 0.63 0.0033
6 0 100 800 90 21.